Kasetsart J. (Nat. Sci.) 40 (Suppl.) : 192 - 197 (2006)
Adsorption of Reactive Dye by Eggshell and Its Membrane Nuttawan Pramanpol and Nuttakan Nitayapat*
ABSTRACT The use of eggshell and its membrane as adsorbents for the removal of reactive dye from aqueous solutions was investigated. The adsorption characteristics of C.I. Reactive Yellow 205 by various components of eggshells were investigated by fitting the experimental data to Freundlich and Langmuir isotherms. Eggshell membranes had a much larger (10 to 27 - fold) capacity to adsorb the dye than did the other components. The initial pH of dye solutions in the range 4-9 did not influence significantly the adsorption of dye by eggshell with membrane and the highest value of adsorption capacity was observed at 35rC. The extent of adsorption of the dye was related directly to the surface area of the adsorbent. The results presented demonstrate clearly that eggshell with its membrane attached is a potentially useful material to be used for the removal of reactive dyes from industrial wastewater. Key words: eggshell, eggshell membrane, reactive dye, adsorption, Freundlich isotherm
INTRODUCTION Large quantities of reactive dyes are utilised by the textile industry. Mainly due to their extensive application in the dyeing of cotton, about 20-30% of all of the dyestuffs used worldwide are reactive dyes. Biodegradation of this group of compounds is significantly slower than that of acid and direct dyes (Zollinger, 2003). The persistent nature of reactive dyes complicates wastewater treatment within the textile industry. Removal of dyestuffs from wastewater occurs by either biological methods or physicochemical methods (e.g., adsorption, oxidation-reduction, chemical coagulation, ozone treatment, and membrane filtration). Removal of reactive dyes by adsorption is one of the many methods widely used. Various adsorbent materials (e.g., activated carbon, chitosan, agricultural waste, and natural waste)
have been studied (McKay, 1996; Batzias and Sidiras, 2004; El Zawahry and Kamel, 2004; Papic et al., 2004; Valix et al., 2004; Zheng et al., 2005; Orfao et al., 2006). Hens’ eggs are used in enormous numbers by food manufacturers and restaurants and the shells are discarded as waste. Many investigations have been conducted to explore useful applications for eggshells. Such research has shown that eggshells may be used as a fertiliser and a feed additive for livestock and it appears to be able to effectively adsorb certain heavy metals and organic compounds (Kuh and Kim, 2000; Koumanova et al., 2002; Chojnacka, 2005; Vijayaraghavan et al., 2005). The porous nature of eggshell makes it an attractive material to employ as an adsorbent. Each eggshell has been estimated to contain between 7000-17000 pores (William and Owen,
Department of Biotechnology, Faculty of Agro-Industry, Kasetsart University 10900, Bangkok, Thailand. * Corresponding author: Email: [email protected]
Received date : 18/04/05
Accepted date : 29/09/06
Kasetsart J. (Nat. Sci.) 40 (Suppl.)
1995). The principal component of the shell is calcium carbonate which comprises more than 90% of the material (William and Owen, 1995; Kuh and Kim, 2000; Stadelman, 2000). The eggshell membrane, which is located between the egg white and the shell, is composed of a network of fibrous proteins that has a large surface area (Tsai et al., 2006). Eggshell membrane has found applications as an adsorbent and as a supporting medium for immobilisation of enzymes. However, the application of discarded eggshells in the removal of reactive dyes by adsorption has received very little attention. This work has been designed to examine the possibility of using eggshell and its membrane as adsorbents for this type of compound. The effects of temperature, pH, and particle size of the adsorbents on the adsorption of a reactive dye were investigated. MATERIALS AND METHODS Reactive Dye C.I. Reactive Yellow 205, a sulphonated reactive azo dye, was obtained from Ciba Specialty Chemicals Inc. Preparation of adsorbents Discarded eggshells were collected from local restaurants. To prevent decomposition, eggshells were first washed in tap water, then boiled in distilled water, and finally dried at 105r C in a hot air oven for 2 h. The membranes were separated from dried eggshells by hand. The dried eggshells and membranes were ground separately using a blender. The powdered materials were sieved to obtain particles of various size ranges. The sieved materials were tested for their adsorbent qualities without further chemical or physical treatment. Adsorption of Reactive Dye by Adsorbents The 50 ml volumes of solutions (pH adjusted to 5.7 with 1M hydrochloric acid)
containing various concentrations of dye were mixed with 2 g of membrane-free eggshell, 2 g of eggshell with membrane, or 0.5 g of eggshell membrane. The size range of the particulate solids was 0.250-0.425 mm. The mixtures were agitated at 35rC using a shaking incubator set at 300 revolutions per minute. Effect of pH on Adsorption of Reactive Dye The pH of 50 ml volumes of solutions containing various concentrations of the dye were adjusted with 1M hydrochloric acid or 1M sodium hydroxide to various values of pH and mixed with 2 g of powdered eggshell with membrane (particle size, 0.250-0.425 mm). The mixtures were incubated at 35rC. Effect of Temperature on Adsorption of Reactive Dye The 50 ml volumes of solutions containing various concentrations of the dye were mixed with 2 g of eggshell with membrane (particle size, 0.250-0.425 mm). The mixtures were agitated at 28, 35, and 40 rC. Effect of Particle Size on Adsorption of Reactive Dye The 50 ml volumes of solutions containing various concentrations of the dye were mixed with 2 g of eggshell with membrane of various size ranges. The mixtures were agitated at 35rC. Determination of Reactive Dye The concentrations of reactive dye in aqueous solutions were determined by measuring the absorbance of the solution at 419 nm using a Shimadzu model UV-1201 spectrophotometer. Aqueous solutions of the dye within the concentration range 0-60 mg/L were used for calibration. Plots of absorbance against concentration were linear. The concentrations of the dye remaining in the aqueous phase of the
Kasetsart J. (Nat. Sci.) 40 (Suppl.)
mixtures were determined periodically until adsorption attained equilibrium. The remaining solids were separated from the liquid phases by centrifugation at 10,000 rpm for 2 min. The experiments were carried out in triplicate. RESULTS AND DISCUSSION Adsorption of Reactive Dye by Adsorbents The various components of eggshell investigated under batch conditions were powdered eggshell devoid of membrane, powdered eggshell with membrane attached, and powdered membrane. Within the range of initial concentrations (20-100 mg/L) of dye investigated, approximately 72% to over 99% of the compound was adsorbed by the various components at equilibrium. The values of qe (amount of dye adsorbed per unit weight of component at equilibrium) are shown in Figure 1. The value of qe for eggshell membrane was much higher than
those for the other two fractions. The data were assessed more closely by considering them in relation to the isotherms of Langmuir (Eqn 1) and Freundlich (Eqn 2), where C, q0 and qe represent the residual (unadsorbed) concentration of dye (mg/L), the maximum amount of dye that can be adsorbed onto the solid matrix (mg/g), and the amount of dye that is adsorbed (mg/g) at equilibrium, respectively. 1/qe = K/q0C + 1/q0 (Eqn 1) qe = KfC1/n (Eqn 2) The term K/q0 gives an estimate of the monolayer adsorbent capacity, q0 being known also as the solute adsorptivity. Kf and n (the Freundlich constants) are indicators of adsorption capacity and adsorption affinity, respectively. When the data were assessed using Freundlich’s isotherm, the logarithmic form of Eqn 2 was employed and log qe was plotted against log C. When the Langmuir’s Eqn was used, 1/qe was plotted against 1/C.
250 eggshell without membrane 200
membrane eggshell with membrane
Initial concentration of dye (mg/L) Figure 1 Adsorption of dye by eggshell components at 35rC
Kasetsart J. (Nat. Sci.) 40 (Suppl.)
All of the plots were linear and the estimates of the various parameters were extracted from the values of their slopes and intercepts. However, better fits to the data were observed much more frequently in the Freundlich plots (Table 1). The values of Kf (adsorption capacity) extracted demonstrated conclusively that eggshell membrane adsorbed the reactive dye much more extensively (10 to 27 – fold) than did the other two fractions (Table 1). Values of n (adsorption affinity) indicated that the membrane had a greater affinity for the dye than did the shell. Tsai et al. (2006) have reported that the properties of the pores of eggshells and the associated membrane are similar and the porosity of the shell is larger than that of the membrane. The results shown in Table 1 and Figure 1 reveal that the eggshell membrane has a much greater adsorption capacity (Kf) and, possibly, adsorption affinity (n) for the reactive dye than the shell. It is concluded, therefore, that adsorption of the dye is not related to the properties of the pores present in these structures. However, the results obtained here indicate that the charged nature of the adsorbing surfaces is the primary mechanism by
which the dye is adsorbed. The reactive dye used contains several sulphonic acid groupings and is negatively charged at the pH of the mixtures employed (pH 7.9–9.2, see Table 2). The eggshell membrane is constructed of a network of fibrous proteins with a surface that bares positively charged sites produced by the basic side chains of the amino acids arginine and lysine. Accordingly, it is not unreasonable to attribute adsorption of the dye involves electrostatic attraction of these oppositely charged species. This idea is supported by the finding that the basic dye methylene blue is very poorly adsorbed by both eggshells and their membranes (Tsai et al., 2006). Effect of pH on Adsorption of Reactive Dye Despite the membranes of eggshells having a substantially greater capacity to adsorb the dye, the procedure for separating this eggshell component is labour intensive and time consuming. Therefore, eggshells with membrane attached were selected for all further investigations. Solutions of dye in water were initially adjusted to pH 4, 7, or 9. Immediately after adding
Table 1 Adsorption of dye onto components of powdered eggshell at 35oC: parameters extracted from Freundlich and Langmuir plots. Freundlich isotherm Langmuir isotherm 2 n Kf r K/q0 q0 r2 Eggshell 1.63 4.89 0.9964 0.2569 48.78 0.9974 Membrane 2.74 131.80 0.9937 0.0007 144.93 0.9516 Eggshell with membrane 2.76 13.09 0.9980 0.0366 30.96 0.9206
Table 2 Adsorption of dye from solutions of various initial pH onto powdered eggshell with membrane: parameters extracted from Freundlich plots. pH of dye solution before Freundlich isotherm pH of Mixtures 2 addition of powdered n Kf r Initially At equilibrium eggshell with membrane 4 2.11 8.81 0.9992 8.7 8.0 7 2.04 8.41 0.9995 8.6 7.9 9 2.22 9.07 0.9991 9.2 8.0
Kasetsart J. (Nat. Sci.) 40 (Suppl.)
eggshells with membrane, the pH of the mixtures observed were 8.7, 8.6, and 9.2 respectively (Table 2) and, at equilibrium, all of the mixtures had very similar values of pH (7.9-8.0, see Table 2). Consequently, all of the Freundlich plots and adsorption parameters generated from the data of these experiments were essentially identical (Table 2). The principal component of the shell is CaCO3 in the form of the mineral calcite. In aqueous solution the carbonate species derived from calcite are H2CO3, HCO3-, and CO32-, the proportions of which are determined by the pH of the resulting solution. The pH of mixtures of eggshell with membrane and solutions of the dye of different initial pH all eventually attained a pH of near 8.0 (Table 2). From this finding it is concluded that sufficient amounts of carbonates are solubilised from the shells to buffer the mixtures to a faintly alkaline pH. Effect of Temperature on Adsorption of Reactive Dye The adsorptions of reactive dye at temperatures of 28, 35 and 40rC were investigated and the relevant values of the Freundlich parameters are displayed in Table 3. There was no obvious relationship between temperature and the adsorption parameters. However, the highest value of adsorption capacity (Kf) was noted at 35rC and temperature appeared to have little effect on adsorption affinity (n).
Table 3 Adsorption of dye onto powdered eggshell with membrane at various temperatures: parameters extracted from Freundlich plots. Temperature Freundlich isotherm (rC) n Kf r2 28 2.00 7.44 0.9991 35 2.71 13.09 0.9980 40 2.24 9.85 0.9983
Effect of Particle Size on Adsorption of Reactive Dye Three different size ranges of particles of adsorbent were examined. The results shown in Table 4, as might be expected, demonstrated clearly that the capacity of the matrix to adsorb the reactive dye is indirectly proportional to its particle size, and, hence, directly related to the surface area of the matrix exposed to the molecules of solute. However, particle surface area did not appear to affect adsorption affinity (n). The results recorded in this study indicate conclusively that the adsorptions of C.I. Reactive Yellow 205 by the components of eggshells take place according to the classical model of adsorption described by Langmuir and Freundlich. However, better fits to the experimental data usually were observed using the logarithmic form of Freundlich’s equation. This observation is not unexpected. It can be explained by considering the nature of the errors associated with the experimental values of qe (the dependent variable). Any small error in q e will become reduced within the term log q e (see Eqn 2) and will become magnified in the value of its reciprocal (see Eqn 1). CONCLUSIONS Powdered membrane has a substantially larger capacity to remove the reactive dye by adsorption than all of the other eggshell
Table 4 Adsorption of dye onto powdered eggshell with membrane for three particle sizes : parameters extracted from Freundlich plots. Particle size Freundlich isotherm range (mm) n Kf r2 0.175 – 0.250 2.23 15.57 0.9951 0.250 – 0.425 2.71 13.09 0.9980 0.425 – 0.850 2.27 10.41 0.9951
Kasetsart J. (Nat. Sci.) 40 (Suppl.)
components. The temperature at which the adsorption occurred and the surface area of the adsorbent influenced markedly the adsorption capacity of eggshells with membrane without having any major effect on its adsorption affinity. Even eggshell devoid of membrane had a significant capacity to adsorb the dye. These results show that eggshell with membrane is a potentially useful material for the removal of reactive dyes from industrial wastewater. It is suggested that work designed to increase the scale of its application to cope with the removal of these compounds under industrial conditions should be initiated. LITERATURE CITED Batzias, F.A. and D.K. Sidiras. 2004. Dye adsorption by calcium chloride treated beech sawdust in batch and fixed-bed systems. J. Hazard. Mater. 114: 167-174. Chojnacka, K. 2005. Biosorption of Cr(III) ions by eggshells. J. Hazard. Mater. 121: 167173. El Zawahry, M.M. and M.M. Kamel. 2004. Removal of azo and anthraquinone dyes from aqueous solutions by Eichhornia crassipes. Wat. Res. 38: 2967-2972. Koumanova, B., P. Peeva, S.J. Allen, K.A. Gallagher and M.G. Healy. 2002. Biosorption from aqueous solutions by eggshell membranes and Rhizopus oryzae: Equilibrium and kinetic studies. J. Chem. Technol. Biotechnol. 77: 539-545. Kuh, S.E. and D.S. Kim. 2000. Removal characteristics of cadmium ion by waste egg shell. Environ. Technol. 21: 883-890. McKay, G. 1996. Use of adsorbents for the removal of pollutants from wastewaters. CRC Press, Boca Raton. 186p.
Orfao, J.J.M., A.I.M. Silva, J.C.V. Pereira, S.A. Barata, I.M. Fonseca, P.C.C. Faria and M.F.R. Pereira. 2006. Adsorption of a reactive dye on chemically modified activated carbons— Influence of pH. J. Colloid. Interface Sci. 296: 480-489. Papic, S., N. Koprivanac, A.L. Bozic and A. Metes. 2004. Removal of some reactive dyes from synthetic wastewater by combined Al(III) coagulation/carbon adsorption process. Dyes Pigm. 62: 291-298. Stadelman, W.J. 2000. Eggs and egg products. In F.J. Francis (ed). Encyclopedia of Food Science and Technology. 2nd ed. John Wiley & Sons. New York. pp.593-599. Tsai, W.T., J.M. Yang, C.W. Lai, Y.H. Cheng, C.C. Lin and C.W. Yeh. 2006. Characterisation and adsorption properties of eggshells and eggshell membrane. Bioresour. Technol. 97: 488-493. Valix, M., W.H. Cheung and G. McKay. 2004. Preparation of activated carbon using low temperature carbonisation and physical activation of high ash raw bagasse for acid dye adsorption. Chemosphere 56: 493-501. Vijayaraghavan, K., J. Jegan, K. Palanivelu and M. Velan. 2005. Removal and recovery of copper from aqueous solution by eggshell in a packed column. Miner. Eng. 18: 545-547. William, J.S. and J.C. Owen. 1995. Egg science and technology. 4th ed. Food Product Press. New York. 590p. Zheng, Y.-M., Q.-B. Zhao and H.-Q. Yu. 2005. Adsorption of a cationic dye onto aerobic granules. Proc. Biochem. 40: 3777-3782. Zollinger, H. 2003. Color Chemistry: Syntheses, Properties, and Applications of Organic Dyes and Pigments. 3rd ed. VHCA/Wiley – Vch. Zurich.